To working surfaces of such steel products for example, saw blade in woodworking the requirements of high wear-resistance at as greater excess as possible in hardness over opposite body of working cutting contact are provided.
Application of diamond grinding with introduction of additional energy as electric discharges diamond-spark grinding in the technologies of reinforced steels allows to raise homogeneity of white layer structures, that will assist to increasing of stability of finished product operation.
Keywords: diamond, friction, microhardness, X-ray, roughness. Introduction The white layer white zones as slightly etching hard buildup, appearing on a surface of steel components during contact thermomechanical influence, for a long time draws attention of researchers from the point of view of possible increase of life-limiting characteristics of operational contact surfaces.
However to the beginning of the third quarter of XX century cautious negative estimations prevailed among metallophysicists as regards practical usage of white layer phenomenon. There is characteristic point of view of worldfamous scientists I.
Lyubarskiy and L. Palatnik : «White zone does not possess satisfactory for effective resistance to deterioration properties, it is frequently formed as separate isolated sites on friction surface or in volume of metal, the non-uniform areas being concentrators of stresses that results in deterioration wear-resistance are formed; the nonequilibrium white zone possesses low fatigue resistance».
Here the same authors in the same work  emphasize: «the problem of white zone is rather actual and wide and demands statement of the further investigations for more detailed studying» citing in author's translation from Russian.
Relaţiile sociale ale militarilor din Dacia romană (II). Căsătoria. ActaMP XXXIII, 2011, p. 159-163
The subsequent investigations of various authors testify to indefatigable temptation to use effect of white layer for the practical purposes. Here we shall note only some examples of successful promotion in this direction. Questions of gc max find find burner efect secundar and purposeful quality management of the processed surface under conditions of white layer formation are investigated by the European technological school .
Achievement of white layer microstructures during electroerosive processing of steel industrial equipment is considered as basic resource of strengthening .
At the Siberian University Russia, Novokuznetsk  even curing of fatigue damages of steels due to electric current pulses and practical technology based on this principle are justified on the basis of the mechanism of formation of local white zones in fatigue cracks.
Method of thermofriction strengthening of steel surfaces, using white layer phenomenon in real embodiments, relieved from the basic disadvantage quoted above on : discontinuity flaw is completely eliminated and substantially - heterogeneity  is developed at Kharkov Polytechnic Institute.
Diamond grinding with introduction of electric current pulses in zone of processing diamond-spark grinding allows both to independently form the strengthened white layers in steels , and to support such layers by means of finishing processing after preliminary thermoclutch strengthening with increase of their uniformity , that holds with electropulse technologies [5,6].
Diamond-spark grinding as finishing postprocessing after thermofriction strengthening Results of research of influence of DSG on phase and stressed state of steels  are evidenced that control of quality of surface layer by means of combining of diamond grinding with sputter ion influence can be more directional including control of forming of both structures of second heat hardening and structures of tempering then in traditional technologies. At that heat of machining surface is a little relative to TFP and it is equivalent to influence of backing, especially under grinding without current and by preliminarily dressed wheel.
Availability of use of diamond-spark grinding on operations of finishing following after thermofriction processing is confirmed of some practice of observation of white layer structures after diamond-spark grinding of steel  that can be explained exclusively thanks to action of electric discharges providing fast impulse heating of machined surface up to phase transformation temperatures.
First International Conference of Thermal Equipment, Renewable Energy and Rural Development
In electric contact patch maximum covering of machined surface in technologies of double speed diamond-spark grinding with increased speeds of working motions of both diamond wheel and machined piece it is to the point of melting and even to partial evaporating, with next enough quick cooling especially under influence of lubricoolant of efficient composition in combination with active technique of supply.
As it marked after known diamond-spark grinding experiment  just combination of high-speed and enough short-term heating with enough quick cooling can provide forming even more so an effective support of qualitative white layer in result of implementation of combined technologies. This hypothesis also proceeds from probable smallness of individual - carbide fragments.
Vray Fast Render Settings In 3ds Max - How To Reduce The render Time In 3dsmax Using V-ray 5 - QA 3
As such fragments there are identified discovered by electron-microscope investigation in near-surface layers of past thermofriction processing steel, moreover on surface of martensate grains, particles of right geometric form with a size approximately µm , that practically is contignous with nanometer excursion, in the case of upper bound of that is taken on a value nm, and with transformation in which of structure of materials are been connected greatest successes of modern hrisca beneficii pt slabit science.
In light of electron-microscope investigations  it is noteworthy that grains carriers of this parts with size µm themselves are more roundish and greatly smaller size about 1 2 µm than size of needled grains of martensite of parent before thermofriction processing texture. Latest research allowed to determine predominant component of white layer microstructure as deformed grainular martensite .
Culturi, procese și contexte în arheologie. 2016 [Cultures, processes and contexts in archaeology]
Conclusions Diamond-spark grinding, especially high-speed processing with cooling, is active mean of support of white layer after thermofriction processing. It is possible efficiently use diamond-spark grinding by combined control of electrical and mechanical operating modes taking into account technical requirements to gc max find find burner efect secundar and roughness, with short-term ironing sparking-out without current if necessary.
References:  Lubarskiy I. Metallophysics of Friction M. The surface integrity of turned and ground hardened bearing steel. Wearpp  Brinksmeter E. White layers in machining steel.
White layer and thermal modeling of hard turned surfaces. Tarel nik, V. Matsinkovskiy, A. Belous, B. Structure Transformations at Electroerosion Treatment of Steels.
- Design Conceptual
- Natalia a crescut pierderea în greutate
- Ion Via; incrowning the long scientific and teaching experience, a paper of the talented prof.
- Analysis of Steam Cracking Process For The Industrial Etylene Plant
- TTMEM English to Romanian glossary of Microsoft terms - Most frequent requests
- Pierderea în greutate la sân înainte și după
- Subject: Re: [Aviatia.
- Pierde în greutate 5kg
Zuev, O. Sosnin, S. Podboronnikov, V. Gromov, S. Journal of Technical Physics,T. Due to measurement and computational tolerances, sufficiently accurate stoichiometric operation requires a closed loop control.
DIAMOND-SPARK GRINDING IN FORMING OF FUNCTIONAL WHITE LAYERS OF INCREASED MICROHARDNESS IN STEELS
Pierdere în greutate eliquis this paper is described the problem of the spark-ignited engine model for lambda control. Keywords: lambda control, platinum, rhodium, pipe. Introduction In SI engines, the air-fuel ration λ is either very lean at load or stoichiometric at medium and high load.
Due to turbulence and local inhomogeneity of the gas mixture, real combustions actually produces HC, CO and NO x at the same time.